Effect of inhibitors on the corrosion of galvanized steel and on mortar properties
Cement & Concrete Composites 35 (2013) 181–189 Contents lists available at SciVerse ScienceDirect Cement & Concrete Composites journal homepage: www.elsevier.com/locate/cemconcompEffect of inhibitors on the corrosion of galvanized steel and on mortar propertiesI. Fayala a,⇑, L. Dhouibi b, X.R. Nóvoa c, M. Ben Ouezdou aa Laboratoire de Génie Civil, ENIT, BP 37 Le Belvédère, 1002 Tunis, Tunisiab Unité de recherche Corrosion et Protection des Métalliques, ENIT, 1002 Tunis, Tunisiac ENCOMAT group, E.T.S.E.I., Universidade de Vigo, 36310 Vigo, Spaina r t i c l e i n f o a b s t r a c tArticle history: This work evaluates two complementary protection methods for steel in concrete: galvanizing coatingReceived 24 June 2012 and corrosion inhibitors. The study was undertaken to evaluate the efﬁciency of using inhibitors (sodiumReceived in revised form 16 August 2012 nitrite, diethanolamine) to protect galvanized reinforcements embedded in mortar against corrosion, andAccepted 18 August 2012 their effect on the mortar properties before and after exposure to chloride environments. Accelerated cor-Available online 30 August 2012 rosion tests were performed on mortar specimens by wet–dry exposure to sodium chloride solution. The electrochemical behavior of rebars was studied using Electrochemical Impedance Spectroscopy; theKeywords: results showed that diethanolamine improves the level of protection of the reinforcement. The inﬂuenceGalvanized steelMortar microstructure of inhibitor additions on mortar properties was considered by characterizing the pore structure usingCorrosion inhibitors Mercury Intrusion Porosimetry and by assessing the dielectric properties of mortar employing ImpedanceImpedance Spectroscopy Spectroscopy. The results revealed that inhibitors addition leads to microstructural changes. DifferentialDifferential Scanning Calorimetry Scanning Calorimetry was applied on mortar samples to elucidate the causes of the observed microstruc-Chlorides exposure tural changes. Ó 2012 Elsevier Ltd. All rights reserved.1. Introduction cracked concrete immersed in seawater and their studies showed the occurrence of pitting corrosion observed at the cracks . Reinforcement corrosion is the most widespread damage mech- Hence, the galvanized steel passivity is lost once chloride contentanism to which reinforced concrete structures are subjected when in the concrete exceeds a threshold concentration which is reportedthey are exposed to aggressive environments. Annual expenditures to be 2% . When reinforced mortar specimens were exposed toto repair corrosion damage are huge. To address this problem, artiﬁcial sea water, galvanized reinforcements abandoned their pas-implementation of corrosion protection systems should be consid- sive state within a few months, after which, corrosion attacks theered when there is a risk of reinforcement corrosion, especially in substrate, yielding a rapid failure of the reinforcement that mightmarine environments. Among the existing protection methods to lead to severe damage and loss of safety of the structure. Thus, galva-improve the corrosion resistance, galvanized reinforcements have nizing seems to be insufﬁcient for long-term durability.been increasingly used as a preventive measure to delay the corro- Moreover, the use of galvanizing as protective method did notsion process of the steel substrate in the presence of aggressive obtain wide acceptance in the past due to the coating reaction withagents such as chloride ions [1–6]. Indeed, the chloride threshold the surrounding aqueous phase of the mortar, yielding a change invalue of zinc is higher than that of ordinary steel reinforcement the bond performance of galvanized bars. Studies performed onbars, so galvanized reinforcement lengthens the service life of this topic present controversial results. The bond loss is attributed,structures exposed to chlorides . according to some authors, to the hydrogen release around the gal- Several studies have established that hot dip galvanized coatings vanized reinforcement and according to others, to the possibleexposed to simulated concrete pore solution develop very stable cor- changes in the mechanical characteristics of steel after galvaniza-rosion products at the coating surface due to the formation of a pas- tion . The contradictory results obtained about bond perfor-sive protective ﬁlm at the interface identiﬁed as hydrozincite . mance of galvanized steel have been attributed to the use ofResults published by different authors on galvanized steel perfor- different types of tests, different cements, and the different agesmance revealed that zinc coating decreased the extent of corrosion of the tested specimens .in sodium chloride exposure compared to ordinary steel . Others Some researchers tried to prevent hydrogen gas evolution by investigated the performance of galvanized steel embedded in applying conversion pre-treatments [14–17]. On the other hand, several researchers deal with the reinforcement corrosion problem by using corrosion inhibitors in the aim to inhibit the onset of chlo- ⇑ Corresponding author. Tel./fax: +216 71875726. ride-induced corrosion of concrete reinforcement. Two issues need E-mail address: email@example.com (I. Fayala).0958-9465/$ - see front matter Ó 2012 Elsevier Ltd. All rights reserved.http://dx.doi.org/10.1016/j.cemconcomp.2012.08.014
182 I. Fayala et al. / Cement & Concrete Composites 35 (2013) 181–189to be addressed in the use of corrosion inhibitors. First and fore- Table 2most is the efﬁciency of inhibiting action which is the most obvi- Mortar specimens tested.ous concern, and second, but of no lesser importance, is the Specimen type Labels Inhibitor contentinﬂuence of this inhibitor on concrete properties. According to Lot no. 1: specimens after 28 days of curingsome researchers  ‘‘an inhibitor adequate to control or to pre- Control specimen S1(C) –vent corrosion of reinforcing steel must be a suitable chemical Specimen with NaNO2 S1(SN) 2%admixture, which when added to concrete in the correct propor- Specimen with DEA S1(DEA) 3.5 L/m3tions, should be able to stop or delay the reinforcement corrosion Lot no. 2: specimens after 28 days of curing + 7 cycles of wet–dry exposure to 3%without adverse effects in the mechanical and physical–chemical NaCl solution Control specimen S2(C) –properties of concrete’’. Reinforced control specimen S2(C,GS) – Many researchers have been interested in the effect of inhibi- Specimen with NaNO2 S2(NS) 2%tors on concrete properties [19–21]. Some authors report that or- Reinforced specimen with NaNO2 S2(NS,GS) 2%ganic inhibitors help to decrease the chloride content in concrete Specimen with DEA S2(DEA) 3.5 L/m3 Reinforced specimen with DEA S2(DEA,GS) 3.5 L/m3and to promote a decrease on the chloride ion diffusion .Unfortunately, none of these two preventive techniques are free The labels shown are those used in the ﬁgures.of shortcomings and present some lacunae. Therefore, the use ofadditional protective measures becomes necessary to protect gal- NaCl solution and 3 days drying in open atmosphere. The experi-vanized reinforcement bars embedded in concrete structures mentation went on up to the 7th wet–dry cycle for unreinforcedagainst corrosion in presence of high chloride concentration. For specimens and to the 12th cycle for reinforced specimens. Unrein-this reason, this study uses two complementary protection meth- forced specimens were cut into slices with 0.86 cm average thick-ods to improve the corrosion resistance of steel reinforcement in ness to be used in the experiment part. The tests were carried outconcrete exposed to marine-type environments: galvanized coat- on triplicate specimens and the average values reported.ing and corrosion inhibitors. The objective of this work is to determine the effects of inhibitoradditions (sodium nitrite and diethanolamine) on the corrosion 3. Experimental resultsresistance of galvanized reinforcing bars and on the mortar proper-ties. A wet–dry cyclic test, which simulates marine environments, 3.1. Electrochemical behavior of galvanized rebarshas been used to evaluate the corrosion behavior of galvanized steel.Those effects are evaluated in terms of polarization resistance for the 3.1.1. Experimental methodgalvanized reinforced specimens and pore microstructure and Electrochemical Impedance Spectroscopy (EIS) tests were car-dielectric properties of mortar samples (permittivity and resistivity). ried out at room temperature (22 ± 2 °C) using a frequency re- sponse analyser and an electrochemical interface by Solartron. The impedance spectra were obtained in the frequency range be-2. Specimens preparation and materials tween 10 mHz and 10 kHz using a three electrodes arrangement. The three electrodes cell consists of a saturated calomel electrode Mortar samples were prepared using Portland cement CEM II/A- as reference electrode (placed perpendicularly to the upper sideL 32.5 N. The chemical composition of the cement used is depicted and on a humidiﬁed sponge piece to establish contact with thein Table 1. reinforced specimen), a stainless steel plate (placed on the upper The sand employed was normalized type, and cement to sand side of the specimen) as counter electrode and the galvanized rebarratio 0.33 was employed. Distilled water was used as mixing water as working electrode (Fig. 1). The working length exposed is 10 cm,with a water-to-cement (w:c) ratio equal to 0.6 in the purpose to the rest of the rebar was masked with epoxy resin. EIS measure-have porous mortar and to accelerate the corrosion process. The ments were performed at the open circuit potential (OCP).corrosion inhibitors considered in this study were sodium nitrite(SN) and diethanolamine (DEA), used as preventive inhibitors. They 3.1.2. Polarization resistance resultswere added to the water, during the mixing phase, in the concen- Polarization resistance, deﬁned as the diameter of the capacitivetration of 2% per weight of cement for SN and in the concentration arc in the complex plane representation of the impedance obtainedof 3.5 L/m3 of mortar for DEA. Smooth ordinary carbon steel rebars at the OCP, was obtained from the EIS spectra at 3, 6 and 12 immer-of 6 mm diameter and 12 cm length were used. Galvanized steel sion cycles (Figs. 2 and 3 illustrate, as an example, the Nyquist plotrebars were produced by hot dip galvanizing process which con- corresponding to the impedance data obtained for S2(DEA, GS)sists in dipping the ordinary carbon steel in molten zinc (450 °C). with detailed spectra and ﬁtting are incorporated to the Fig. 3).Specimens of (40 Â 40 Â 160 mm) were made by casting the mor- The results of polarization resistance values obtained are summa-tar in prismatic molds. After 24 h, the specimens were demoulded rized in Fig. 4. It can be noticed that SN addition produces lowerand cured for 28 days in distilled water to ovoid any contamina- polarization resistance values than those corresponding to thetion. Reinforced specimens were also manufactured by embeddinga galvanized rebar in the in the center of the specimen, with 1.7 cmmortar cover. As can be seen in Table 2, some of these specimens (lot no. 2)were submitted, after the curing period, to alternate wetting anddrying in sodium chloride solution in order to accelerate chloridepenetration. One cycle consists of 3 days immersion in 3%Table 1Chemical composition of the cement, according to the producer. Oxydes SiO2 Al2O3 Fe2O3 CaO MgO SO3 K2O Fig. 1. The three electrodes arrangement used to perform EIS measurements on Content (%) 17.38 3.86 3.22 60.75 1.26 2.41 0.74 reinforced specimens.
I. Fayala et al. / Cement & Concrete Composites 35 (2013) 181–189 183 40 3 cycles 35 6 cycles 12 cycles 30 25 20 15 10 5 0 S2(C, GS) S2(NS,GS) S2(DEA,GS) Type of the specimenFig. 2. Nyquist plot corresponding to the impedance data obtained for reinforcedmortar specimens with DEA addition (3.5 L/m3) after 3, 6 and 12 cycles of wet–dry Fig. 4. Evolution of polarization resistance values obtained for reinforced mortarexposure to 3% NaCl solution. specimens after 3, 6 and 12 cycles of wet–dry exposure to 3% NaCl solution.control sample. Moreover, after 12 cycles the Rp values fall below On the other hand, the DEA addition increases clearly the polar-the kX scale, which means very high corrosion rate. ization resistance value after the 6th cycle of wet–dry exposure. (a) (b) (c) 60 S2(DEA,GS) 12 cycles 50 fitted data 40 2 - Z Im / kOhm.cm 30 25 30 20 20 15 10 10 5 0 0 5 10 15 20 0 0 10 20 30 40 50 60 2 Z Re / kOhm.cmFig. 3. Nyquist plot corresponding to the impedance data obtained for reinforced mortar specimens with DEA addition (3.5 L/m3): (a) after three cycles, (b) after six cycles and(c) after 12 cycles of wet–dry exposure to 3% NaCl solution.
184 I. Fayala et al. / Cement & Concrete Composites 35 (2013) 181–189 (a) 60 100 nm (b) 55 S1(C) [19,9%] 70 S1(SN) [21%] S1(C) 50 S1(DEA) [18%] S1(SN) -1 60 Incremental volume / µl.g 45 S1(DEA) >100 nm 40 50 10 nm Contribution % 35 30 40 25 30 20 15 20 10 10 5 0 0 0 1 2 3 4 5 6 10 nm 100 nm > 100 nm 10 10 10 10 10 10 10 Pore size / nm Pore diameter / nm Sample S1(C) S1(SN) S1(DEA) Total porosity 19.9 21.0 18.0 Family 1 : (> 100 nm) 61.03 64.16 52.97 Family 2 : (100 nm) 25.54 22.27 32.90 Family 3 : (10 nm) 13.43 13.57 14.13Fig. 5. Mercury Intrusion Porosimetry results corresponding to mortar samples after 28 days curing. (a) Incremental volume of mercury intruded as a function of porediameter. The total porosity is also indicated in the legend. The three groups of pore families analysed are indicated; (b) relative contribution to total porosity of the three porefamilies chosen in (a). Furthermore, in order to validate the obtained results, the mor- 3.2.2. Microstructure analysistar specimens were examinated after 12 wet–dry cycles by visual The hydration reactions induce the development of intercon-evaluation. This was performed by observing the state of the galva- nected pores of different sizes. The pores can be divided into mac-nized bars after splitting the specimens. The galvanized coating, for ropores, capillary pores and gel pores. The capillary pores are thethe specimens S2(C,GS) and S2(SN,GS), was totally dissolved and voids not ﬁlled by the solid products of hydration. In determiningthe state of the reinforcement became similar to an ordinary car- the role of the mortar in protecting the embedded galvanized rein-bon steel. However, the reinforcement in the specimen S2(DEA,GS) forcements, not only should the total capillary porosity (i.e. thehad an aspect similar to that observed for the control specimen but percentage of volume occupied by capillaries) be considered butwith the presence of some local zones which conserved a galva- also the size and the interconnections of capillary pores.nized coating. These results revealed the performance of DEA when The experimental results of the microstructure analysis are pre-it is added to mortar to protect galvanized steel reinforcement sented in pore size logarithmic scale, as can be seen in Figs. 5a andagainst corrosion in the case of accelerated corrosion tests. The 6a, which show the pore size distribution and the total porosity ob-use of this inhibitor can be quite efﬁcient to protect galvanized tained for the tested specimens. Figs. 5b and 6b illustrate the rela-steel reinforcements in concrete structures exposed to marine tive contribution to total porosity of the three pore families chosenenvironments. in the purpose to compare the effect of inhibitor addition on mor- tar microstructure before and after chloride exposure. MIP performed for samples issuing from specimens after curing3.2. Mercury Intrusion Porosimetry (MIP) period (Fig. 5) reveals that inhibitor addition did not affect the frac- tion of smallest pores (10 nm); it is about 15% for the three sam-3.2.1. Experimental method ples. However, an increase of the fraction of larger pores and a MIP was employed for microstructure characterization. This decrease of medium size pores were found when SN is used com-technique enables us to obtain valuable information on pore pared to the control sample. But, the addition of DEA seems to de-structure. crease the fraction of larger pores (>100 nm) to develop smaller The porosimeter utilised was an AUTOPORE IV 9500 from pores, which suggests the formation of a large number of intercon-Micromeritics that measures pore diameters from 0.9 mm down nections between larger size pores. This phenomenon will lead toto 5 nm thanks to the maximum yield pressure of 227 MPa. In increasing both pore tortuosity and percolation, being responsiblethe purpose to make the measuring sample representative of the to the decreasing of the total porosity for samples with DEAreal pore structure, samples with irregular random shapes were addition.cut from the slices . It can be noticed from MIP results performed on samples issuing In the ﬁrst step of the experiment, there is a stage of air evacu- from specimens after wet–dry exposure (Fig. 6) that chloride expo-ation where the pressure reaches 50 lmHg in the recipient holding sure increases the fraction of smallest pores (10 nm), it is aboutthe sample in order to evacuate air and moisture in the pores. The 20% for the three specimens. The microstructure of S2(SN) resem-second step consists in ﬁlling up the recipient with mercury and ﬁ- bles to the control sample S2(C). However, the exposure to chloridenally, pressures are applied to the sample. The more the pressure environment of S2(DEA) engenders a small fraction of medium sizeincreases, the more the diameter of investigated pore is small. pores and increases the fraction of larger pores without affectingMIP was performed for samples issuing from specimens after cur- the total porosity of the sample (15.8% compared to 15% foring period and others after the wet–dry exposure to the sodium S2(C)). The decreasing of total porosity for all the samples S2(C),chloride solution. S2(SN) and S2(DEA) is due to the formation of Friedel’s salt (the
I. Fayala et al. / Cement & Concrete Composites 35 (2013) 181–189 185 (a) 50 (b) S2(C) [15%] 60 45 100 nm S2(SN) [18%] S2(C) S2(DEA) [15,8%] -1 40 S2(SN) Incremental volume / µl.g 50 S2(DEA) 35 Contribution % 10 nm 40 30 >100 nm 25 30 20 15 20 10 10 5 0 0 0 1 2 3 4 5 6 10 nm 100 nm > 100 nm 10 10 10 10 10 10 10 Pore size / nm Pore diameter / nm Sample S2(C) S2(SN) S2(DEA) Total porosit ty 15.0 18.0 15.8 Family 1 : (> 100 nm) 52.58 53.29 57.17 Family 2 : (100 nm) 25.96 27.55 22.83 Family 3 : (10 nm) 21.46 19.16 20.00Fig. 6. Mercury Intrusion Porosimetry results corresponding to mortar samples after 28 days curing and seven cycles of wet–dry exposure in a 3% NaCl solution. (a)Incremental volume of mercury intruded as a function of pore diameter. The total porosity is also indicated in the legend. The three groups of pore families analysed areindicated; (b) relative contribution to total porosity of the three pore families chosen in (a).reaction of cement’s C3A phase and chloride ions) which is a lay-ered structure of calcium aluminates stabilized by chlorides andwater, and occupying the interlamellar spaces. EDX and XRD anal-ysis performed on mortar samples saturated with NaCl 1 M solu-tion conﬁrmed this hypothesis . But, the inﬂuence of Friedel’ssalts on the mortar microstructure for specimens containing inhib-itors differs from the control sample; the reaction seems to bedependent on the inhibitor addition.3.3. Impedance Spectroscopy (IS)3.3.1. Experimental method Fig. 7. Flat cell employed for impedance measurements (schematic). Electrodes are126.96.36.199. Mortar permittivity. The IS measurements were performed, circular, £ 40 mm.from 15 MHz down to 10 kHz, using an HP 4194A impedance gain/phase analyser. Capacitance measurements can be performed inthe range of 10À14–0.1 F with a maximum resolution of 10À14 F. 4194A impedance gain/phase analyser used before in the high fre-A non-contacting method, used previously in others studies quency range (10 kHz–15 MHz). The sample’s resistivity assess-[22,24,25], was employed by means of the HP 16451B Dielectric ment enables us to take into account the diffusion eventualityTest Fixture (Fig. 7). This method minimizes the possible contribu- via percolating capillary porosity. Resistivity is an importanttion of the sample–electrode interface. It consists of leaving an air parameter assessed in the aim to supply information on the watergap between sample and electrode or by placing polyester sheets content in the mortar, the resistance to chloride penetration or the(100 lm thick) to insulate the electrodes. The impedance of the corrosion rate.air gap was measured prior to the samples measurement and Before testing, the mortar samples were pre-conditioned by sat-numerically subtracted from the overall impedance after measure- uration with NaCl 1 M solution . Samples were kept in the ﬁll-ment, to obtain only the impedance of the sample. ing solution until performing the measurements. The electrodes employed were high density sheets of graphite. The resistivity is calculated from the resistance value (R1) mea-Before testing, samples were left at laboratory atmosphere for nat- sured between the electrodes (obtained from Nyquist plots) byural drying. Then, they were held on vacuum machine to get water means of the following equation:evaporation without causing morphological changes. The dielectric R1 Â Sconstant of the mortar sample is given by the following equation: q¼ ð2Þ e e Â C1e¼ ð1Þ where q is the resistivity (X m), R1 is the measured resistance be- e0 tween electrodes (X), S is the exposed surface of the mortar samplewhere C1 is the calculated dielectric capacitance (F cmÀ2), e is the to the chloride solution (corrected for the electric ﬁeld dispersionsample thickness (cm) and e0 is the vacuum permittivity ), e is the sample thickness.(8.85 Â 10À14 F cmÀ1). 3.3.2. Mortar dielectric properties188.8.131.52. Mortar resistivity. The IS measurements were carried out As it can be seen in Fig. 9, the impedance of the sample is capac-using the arrangement shown in Fig. 8 connected to the HP itive, so the Cole–Cole transformation (Eq. (3)) is used with the aim
186 I. Fayala et al. / Cement & Concrete Composites 35 (2013) 181–189 Fig. 8. Arrangement used to determine mortar’s resistivity by Impedance Spectroscopy. Fig. 11. Cole–Cole plot corresponding to impedance data given in Fig. 7 obtained for the control sample after seven cycles of wet–dry exposure to chloride solution. Table 3Fig. 9. Nyquist plot corresponding to the impedance data obtained for the control Summary of Impedance Spectroscopy results for mortar specimens.sample after seven cycles of wet–dry exposure to chloride solution. e C1 C2 fm R2 e (cm) (pF cmÀ2) (pF cmÀ2) (MHz) (kX cmÀ2) Lot no. S1(C) 0.89 7.9 14.1 0.88 1284.7 7.9 1 S1(SN) 0.86 8.0 10.0 1.91 833.7 7.8 S1(DEA) 0.88 8.5 11.6 1.63 842.2 8.5 Lot no. S2(C) 0.89 8.8 18.9 0.52 1604.8 8.9 2 S2(SN) 0.85 7.5 12.0 0.90 1461.4 7.2 S2(DEA) 0.87 8.4 12.3 1.17 1106.5 8.3 C2 CðxÞ ¼ C 1 þ ð4Þ ð1 þ ðjxR2 C 2 Þa ÞbFig. 10. Schematic representation of the equivalent circuit model employed forﬁtting high frequency impedance data corresponding to mortar using the non-contacting method. C1 represents the solid phase contribution, and R2 and C2 are where the a and b parameters are constants, 0 < a, b 6 1, that ac-attributed to the electrolyte ﬁlling the pores . count respectively for the symmetric (Cole–Cole) and asymmetric (Cole–Davidson) dispersion of the R2C2 time constant. The high frequency limit of the Cole–Cole plot, C1, is deﬁned by the dielectric capacitance of the solid phase in the mortar while theof accurate representations, which have well deﬁned high and low capacitance, C2, deﬁnes the low frequency limit of the complexfrequency limits. C(x) is the complex capacitance and Z(x) the capacitance plot (C1 + C2) and it is directly linked to the doubleimpedance of the sample at angular frequency x . layer capacitance formed at the C–S–H gel layers limiting occupied 1 pores. C2 and the resistance R2 are parameters associated to theCðxÞ ¼ ð3Þ contribution of the liquid phase ﬁlling pores. Subsequently, these jxZðxÞ parameters have both a strong dependence on the amount of water The Cole–Cole representation, which is a complex capacitance in the sample as well as on pore structure .plot, is considered as the simplest way of studying the dielectric The obtained dielectric parameters C1, C2 and R2 are depicted inbehavior of mortar. Table 3. The capacitance C1, obtained from the plot, enables us to An example of the Cole–Cole transformation of data presented calculate the apparent dielectric constant of the mortar samplein Fig. 9 is depicted in Fig. 11. The equivalent circuit model , which is proportional to the fraction of solid phase presentemployed for ﬁtting impedance data is depicted in Fig. 10. The rep- in the system (compactness degree).resentation depicted in Fig. 11 corresponds to a typical The data reported in Table 3 are in good agreement with theCole–Davidson dispersion shape that can be modeled using the MIP results. For the cured samples (Fig. 3, lot no. 1 in Table 3) itfollowing equation : can be seen that samples with DEA addition present the lower
I. Fayala et al. / Cement & Concrete Composites 35 (2013) 181–189 187porosity (18%) and also higher apparent dielectric constant (com-pactness). Changes in the porosity distribution are related to theR2C2 time constant, which decreases in presence of the inhibitors(the characteristic frequency increases). Moreover, the decreasedR2 values for the mixes containing the inhibitors suggest an in-creased conductivity of the pore electrolyte. For the lot no. 2, the lowest apparent dielectric constant corre-sponds to the samples with SN addition, in accordance with the to-tal porosity value reported in Fig. 6 were those samples show thehighest porosity. The effect of the Friedel’s salt precipitation is evi-dent in the R2C2 time constant: R2 increases with respect to theunexposed samples, and C2 increases too due to increased tortuos-ity of the pore network.3.3.3. Mortar resistivity The equivalent circuit in this case is depicted in Fig. 12. The onlydifference with the one used in the previous section (Fig. 10) is theadditional parameter, R1, which accounts for sample’s resistivityi.e., resistance associated to percolating pores [23,25]. So, the resis-tivity is related to the conductivity of the solution ﬁlling pores(resistivity increases as the ionic concentration of this solution de-creases). Fig. 13 corresponds to the normalized impedance corre- Fig. 13. Normalized impedance spectrum (Nyquist plot) corresponding to thesponding to the mortar sample S2(SN). R1 corresponds to the mortar sample with 2% sodium nitrite addition after seven cycles of wet–drydiameter of the high frequency capacitive arc in Fig. 13. The low exposure to chloride solution used to obtain the mortar resistivity.frequency contribution (below 1 MHz) corresponds to theelectrodes. As expected (see Table 4), the mortar resistivity correlates well Table 4 Mortar resistivity values.with the conductivity of the solution ﬁlling pores: resistivity valueincreases when mortar sample is submitted to wet–dry cyclic test. Specimen e (cm) R1 (X) q (X cm)Thus, it can be said that during the wetting period chloride ions Lot no. 1 S1(C) 0.87 2250 2030penetrate in capillary pores and form Friedel’s salt which clinged S1(SN) 0.89 2100 1852to the pore surface during the drying period. The resistivity in- S1(DEA) 0.86 3508 3202creases with the hydration of the cement. A decrease of the resis- Lot no. 2 S2(C) 0.87 3760 3392tivity value explains an increase of the amount of water-ﬁlled S2(NS) 0.86 3214 2934 S2(DEA) 0.87 4500 4060pores. An increased resistivity is accompanied by a reduced corro-sion rate . The increasing of the mortar resistivity in presence of DEA re-veals the performance of this inhibitor to improve the hydration The DSC tests were performed on specimens of lot no. 1 usingprocess of the mortar. Indeed, this result can be explained by the an 822 Mettler Toledo calorimeter with a computer-controlled fur-decreasing of the amount of water ﬁlling pores. It is well known nace. The samples were heated in the range 25 up to 700 °C at athat a high resistivity value means a better corrosion resistance constant rate (10 °C/mn) in a dynamic nitrogen atmosphereof the material because of the improved barrier properties. Thus, (20 ml/mn). This method of thermal analysis was applied to inves-DEA can be considered as a good corrosion inhibitor for steel rein- tigate the effect of inhibitor addition on the process of cementforcements with respect to the control sample. However, results hydration and to identify the formation of dehydrated and trans-obtained in the presence of SN clearly show the inefﬁciency to pro- formed phases of mortar samples. The analysis was performed ontect reinforcements when they are embedded in mortar. mortar samples taken from portions in the middle of the mortar slices. DSC curves of mortar specimens are shown in Fig. 14. The samples used weighted around 30 mg.3.4. Differential Scanning Calorimetry (DSC)3.4.1. Experimental method 3.4.2. DSC results Thermal analysis has proved to be a valuable technique in the Fig. 14 shows the DSC curves obtained for mortar samples afterstudy of cement hydration [29,30]. DSC is considered as an impor- 28 days. These curves are plotted with the endothermal behaviortant tool for evaluating the nature of hydrated products. in the downward direction, as is the convention in most of the ce- ment and concrete literature. A number of peaks were observed and these curves can be divided into ﬁve major parts, according to different reactions: 25–115 °C: dehydration of pore water. 115–420 °C: different stages of C–S–H dehydration. 420–480 °C: dehydroxylation of Ca(OH)2. 480–600 °C: conversion of SiO2. 480–700 °C: decarbonation of CaCO3.Fig. 12. Schematic representation of the equivalent circuit employed to model the From 25 to 200 °C, the free water and a part of the bound waterdata corresponding to saturated mortar samples with NaCl 1 M solution . of hydrated products escape such as C–S–H gel  and the
188 I. Fayala et al. / Cement Concrete Composites 35 (2013) 181–189 Fig. 14. Differential Scanning Calorimetry curves of mortar samples after 28 days of curing.decomposition of ettringite takes place . Indeed, the peak be- It can be also noticed the existence of a clear dependence be-fore 100 °C corresponds to the C–S–H gel dehydration. tween permittivity values and the samples porosity. The permittiv- The C–S–H peak, occurring at around 140 °C, is increased with ity evolution mimics the evolution of the total porosity: thethe use of DEA. The peak observed at 175 °C corresponds to the sample’s permittivity increases as the porosity decreases. In a pre-ettringite, resulting from the reaction between C3A and gypsum vious study  on cement paste hardening process, researchers(gypsum is added in ordinary Portland cement to avoid the fast obtained a linear dependence of permittivity with w:c ratio. Ashydration of C3A). for given cement paste the w:c ratio determines its porosity, per- Up to 400 °C, the bound water is lost in C–S–H gel, which is mittivity measurements can provide a fast method of real timetransformed into a modiﬁed C–S–H and partially dehydrated C– evaluation of the sample’s porosity.S–H with low crystalline structure [31,33]. The porosity increasing decreases the volume fraction of solid At 576 °C, the peak is similar for all mortar samples; it is due to phase and hence the associated capacitance values decrease too.the conversion of quartz (SiO2) in the sand . This effect can DEA seems to react with hydration products. The reaction withcause a volume expansion and make the sand broken. Ca(OH)2 results in a gel formation that block the pores of the mor- All curves show an exothermic peak in the vicinity of 450 °C, it tar. The pore-blocking effect is a secondary property as it causes acorresponds to the dehydroxylation of portlandite (decomposition reduction in the chloride ingress into mortar. Subsequently, theof Ca(OH)2 to CaO and H2O), another hydration product , but corrosion process is delayed.this peak is less intense for mortar sample containing SN indicating Another interesting feature concerns the inhibitors effect on theless Ca(OH)2 content. It is known that SN is slight acid and can neu- hydration process of mortar samples. From the Calorimetry inves-tralize calcium hydroxide. X-ray analysis conﬁrmed the absence of tigations performed, showed in the DSC curves, it is possible toCa(OH)2 in DSC samples heated to 635 °C. And the peak at 670 °C conclude that inhibitors did not inﬂuence generally the cementcorresponds to the decarbonation of calcium carbonate . hydration, but, it is clearly shown that there is a modiﬁcation in Continuously heating to 700 °C, the decarbonation of calcium the stages of C–S–H dehydration especially with the addition ofcarbonate and the complete dehydroxylation of calcium hydroxide DEA.occur [34,35]. In addition, the C–S–H gel completely changes into It’s also clear that the addition of SN modiﬁed the dehydroxyla-dehydrated C–S–H . tion of portlandite process (decomposition of Ca(OH)2 to CaO and H2O) shown in the peak in the vicinity of 450 °C. This is owing to4. Discussion the acidity of SN which causes the neutralization of calcium hydroxide i.e. less Ca(OH)2 content. This inﬂuence corroborate The results presented above reveal the effect of the DEA as a the results obtained for the total porosity (21%) of the specimenscorrosion inhibitor for steel in concrete is twofold: direct and indi- S1(SN) which can explain the negative effect when specimens wererect. The direct action concerns the faradaic process that is hin- exposed to chloride environment. However, the use of DEA did thedered in presence of the amine, as the polarization results reveal. opposite effect on the dehydroxylation of portlandite processThe indirect action concerns the barrier-forming effect because it which can explain less porosity (18%) and then a good performancedecreases the porosity of the concrete and increases resistivity. in presence of chlorides with respect to the control specimens. Dielectric properties clearly reﬂect the pore structure develop-ment and the degree of pore occupancy by electrolyte. 5. Conclusions MIP results show also that the microstructure of mortar evolvesin presence of chlorides, mainly due to the formation of Friedel’s The above-discussed results reveal interesting aspects of usingsalts. Overall porosity changes, new pore families develop and galvanized coating and inhibitor addition. In particular, these twopore’s tortuosity too. preventive methods act in a complementary manner to delay cor- The variations in R2 values are closely related to the hydration rosion: galvanizing protects the steel reinforcement and the inhib-process of the mortar. The hydration involves the reaction of C3- itor reacts with mortar by improving its performance in presenceS(3CaOSiO2) and C2S(2CaOSiO2) with free water to form calcium of chloride environment.silicate hydrate (C–S–H) and calcium hydroxide . These reac- The evolution of polarization resistance values, measured ontions promote the formation of a rigid microstructure and strength reinforced mortar specimens after 3, 6 and 12 cycles of wet–drydevelopment. exposure to 3% NaCl solution, show that the corrosion resistance
I. Fayala et al. / Cement Concrete Composites 35 (2013) 181–189 189of galvanized rebars is improved in presence of DEA with respect to  Fratesi R. Galvanized reinforcing steel bars in concrete. COST 521 workshop, Luxembourg; 2002.the control specimen, contrary to the use of SN which accelerates  Comité Euro-International de Béton (CEB). Protection systems forthe corrosion process. reinforcement. Bulletin d’information No. 211, 1992, Paris. Impedance measurements in the frequency range (10 kHz–  Montemor MF, Simões AM, Ferreira MGS. Composition and corrosion15 MHz) can supply information on pore network development behaviour of galvanised steel treated with rare-earth salts: the effect of the cation. Prog Org Coat 2002;44(2):111–20.as well as on pore occupancy; these measurements, with Mercury  Ferreira MGS, Duarte RG, Montemor MF, Simões AMP. Silanes and rare earthIntrusion Porosimetry results corresponding to mortar samples salts as chromate replacers for pre-treatments on galvanised steel.after 28 days curing, showed that the inhibitor addition inﬂuenced Electrochim Acta 2004;49(17–18):2927–35.  Trabelsi W, Cecilio P, Ferreira MGS, Montemor MF. Electrochemicalthe microstructure and the pore distribution of the mortar (a de- assessment of the self-healing properties of Ce-doped silane solutions forcrease of the total porosity with the DEA and an increase of total the pre-treatment of galvanised steel substrates. Prog Org Coatporosity with the SN). These changes were explained by the effect 2005;54(4):276–84.  Sánchez M, Alonso MC, Cecílio P, Montemor MF, Andrade C. Electrochemicalof the inhibitor on the components of the mortar, especially the ef- and analytical assessment of galvanized steel reinforcement pre-treated withfect on the dehydroxylation of portlandite process shown by the Ce and La salts under alkaline media. Cem Concr Compos 2006;28(3):DSC results. 256–66.  Jamil HE, Shriri A, Boulif R, Bastos C, Montemor MF, Ferreira MGS. The above discussed results show also that the microstructure Electrochemical behaviour of amino-alcohol-based inhibitors used to controlof mortar evolves in presence of chlorides (mainly due to the for- corrosion of reinforcing steel. Electrochim Acta 2004;49(17–18):2753–60.mation of Friedel’s salts). Overall porosity changes, new pore fam-  Buffenbarger JK, Miltenberger MA, Miller BD, Casal HL. Long term performance of organic inhibitors. In: Proceedings of the international congress onilies develop and pore system tortuosity also changes. There exists advanced materials, their process and applications, Munich, September 2000.a clear dependence between permittivity values and sample poros-  Brown MC, Weyers RE, Sprinkel MM. Effect of corrosion-inhibiting admixturesity. The permittivity evolution mimics the evolution of the total on material properties of concrete. ACI Mater J 2001;98(3):240–50.porosity: the sample’s permittivity increases as the porosity  De Schutter G, Luo L. Effect of corrosion inhibiting admixtures on concrete properties. Constr Build Mater 2004;18(7):483–9.decreases.  Cabeza M, Keddam M, Nóvoa XR, Sánchez I, Takenouti H. Impedance The results obtained in this work clearly show that the corro- spectroscopy to characterize the pore structure during the hardeningsion behavior of galvanized steel in reinforced mortar specimens process of Portland cement paste. Electrochim Acta 2006;51(8–9): 1831–41.is greatly improved by the addition of DEA, which acted as an efﬁ-  Díaz B, Freire L, Merino P, Nóvoa XR, Pérez MC. Impedance spectroscopy studycient corrosion inhibitor in chloride environment by inﬂuencing of saturated mortar samples. Electrochim Acta 2008;53(25):7549–55.the microstructure of the mortar.  Keddam M, Takenouti H, Nóvoa XR, Andrade C, Alonso C. Impedance measurements on cement paste. Cem Concr Res 1997;27(8):1191–201.  Cabeza M, Merino P, Miranda A, Nóvoa XR, Sanchez I. Impedance spectroscopyReferences study of hardened Portland cement paste. Cem Concr Res 2002;32(6): 881–91.  Macias A, Andrade C. The behaviour of galvanized steel in chloride-containing  ASTM Standard C 1202-97. Standard test method for electrical indication of alkaline-solutions. I: The inﬂuence of the cation. Corros Sci 1990;30(4– concrete’s ability to resist chloride ion penetration, Annual Book of ASTM 5):393–407. Standard, Section 4, vol. 04.02, 2000.  Yeomans SR. Performance of black, galvanized and epoxy-coated reinforcing  Díaz B, Freire L, Nóvoa XR, Puga B, Vivier V. Resistivity of cementitious steels in chloride-contaminated concrete. Corrosion 1994;50(1):72–81. materials measured in diaphragm migration cells: the effect of the  Bautista A, Gonzalez JA. Analysis of the protective efﬁciency of galvanizing experimental set-up. Cem Concr Res 2010;40(10):1465–70. against corrosion of reinforcements embedded in chloride contaminated  Andrade C, Blanco VM, Collazo A, Keddam M, Nóvoa XR, Takenouti H. Cement concrete. Cem Concr Res 1996;26(2):215–24. paste hardening process studied by impedance spectroscopy. Electrochim Acta  Ramirez E, Gonzalez JA, Bautista A. The protective efﬁciency of galvanizing 1999;44(24):4313–8. against corrosion of steel in mortar and in Ca(OH)2 saturated solutions  Bhatty JI. A review of the application of thermal analysis to cement–admixture containing chlorides. Cem Concr Res 1996;26:1525–39. systems. Thermochim Acta 1991;189(2):313–50.  Belaid F, Arliguie G, François R. Corrosion products of galvanised rebars  Abdelrazig BEI, Main SD, Nowell DV. Hydration studies of modiﬁed OPC pastes embedded in chloride-contaminated concrete. J Sci Eng Corros by differential scanning calorimetry and thermogravimetry. J Therm Anal 2000;56(9):960–5. 1992;38(3):495–504.  Yeomans SR, editor. Galvanized steel reinforcement in concrete. Elsevier; 2004.  Alarcon-Ruiz L, Platret G, Massieu E, Ehrlacher A. The use of thermal analysis in  Darwin D, Browning J, O’Reilly M, Xing L, Ji J. Critical chloride corrosion assessing the effect of temperature on a cement paste. Cem Concr Res threshold of galvanized reinforcing bars. ACI Mater J 2009;106(2):176–83. 2005;35(3):609–13.  Ghosh R, Singh DDN. Kinetics, mechanism and characterization of passive ﬁlm  Castellote M, Alonso C, Andrade C, Turrillas X, Campo J. Composition and formed on hot dip galvanized coating exposed in simulated concrete pore microstructural changes of cement pastes upon heating, as studied by neutron solution. Surf Coat Technol 2007;201(16–17):7346–59. diffraction. Cem Concr Res 2004;34(9):1633–44.  Okamura H, Hisamatsu Y. Effect of use of galvanized steel on the durability of  Alonso C, Fernandez L. Dehydration and rehydration processes of cement paste reinforced concrete. Mater Perform 1976;15(7):43–7. exposed to high temperature environments. J Mater Sci 2004;39(9):3015–24. Fratesi R, Moriconi G, Coppola I. The inﬂuence of steel galvanization on rebars  Grattan-Bellew PE. Microstructural investigation of deteriorated Portland behaviour in concrete. In: Page CL, Bamforth PB, Figg JW, editors. Corrosion of cement concretes. Constr Build Mater 1996;10(1):3–16. Reinforcement in Concrete Construction. Royal Society of Chemistry; 1996. p.  Handoo SK, Agarwal S, Agarwal SK. Physicochemical, mineralogical, and 630–41. morphological characteristics of concrete exposed to elevated temperatures. Swamy RN. Resistance to chlorides of galvanized rebars. In: Page C, Treadaway Cem Concr Res 2002;32(7):1009–18. KWJ, Bamforth PB, editors. Corrosion of Reinforcement in Concrete. London,  Taylor HFW. Hydration of the calcium silicate phases, cement chemistry. 2nd New York: Elsevier Appl. Sci; 1990. p. 586–600. ed. London: Thomas Telford Publishers; 1998. p. 113 [chapter 5].